A thermal weld study was conducted on various gauges of PVC for the purpose of identifying a temperature windows in which PVC could be welded.
The material test strips used were 20 mil PVC, 30 mil PVC, and 40 mil PVC; manufactured by Occidental Chemical Corporation and thermally welded with a dual track seam.
The mouse type welder was used utilizing a split wedge. The welded area consisted of two ½" welds with a ½" air channel in between. The liner welder is adjustable from 0 to 10 feet per minute for the travel speed, and 0 to 500 degrees Celsius for the wedge temperature. The constant speed used for this test was 7 feet per minute, and the wedge temperature was started at 100° Celsius and increased at 25° intervals until the material fused together, and continued incrementally up to 425° , or until a point at which the weld becomes unacceptable.
A sample strip of sufficient length, (approximately 100 feet) was prepared of each of the three materials. Once the weld occurred at the lower Temperature, a 16" sample could be fabricated at each 25° interval from the lowest to the highest weldable temperature. The ambient room temperature for fabrication of these test strips was 21° Celsius, and the humidity was 64%.
Five specimens of each temperature range sample were removed for peel testing per NSF-54. The average of the five specimens from each sample were recorded on a graph. Each material type is shown on the accompanying graph.
The graph illustrates the wedge window for all three thicknesses of PVC would be 250° Celsius to 375° Celsius. Although the window for some thicknesses may be larger than the three combined, the ultimate goal was to establish the range of temperatures for wedge welding PVC.
For more information call 800-OK-LINER today!